||This article needs additional citations for verification. (October 2011)|
Pulp produced by the kraft process is stronger than that made by other pulping processes; acidic sulfite processes degrade cellulose more, leading to weaker fibers, and mechanical pulping processes leave most of the lignin with the fibers, whereas kraft pulping removes most of the lignin present originally in the wood. Low lignin is important to the resulting strength of the paper as the hydrophobic nature of lignin interferes with the formation of the hydrogen bonds between cellulose (and hemicellulose) in the fibers.
Kraft pulp is darker than other wood pulps, but it can be bleached to make very white pulp. Fully bleached kraft pulp is used to make high quality paper where strength, whiteness and resistance to yellowing are important.
Wood pulp for sack paper is made from softwood by the kraft process. The long fibers provides the paper its strength and is added wet strength chemicals to even further improve the strength. Both white and brown grades are made. Sack paper is then produced on a paper machine from the wood pulp. The paper is microcrepped to give porosity and elasticity. Microcrepping is done by drying with loose draws allowing it to shrink. This is causing the paper to elongate 4% in machine direction and 10% in cross direction before busting. Machine direction elongation can be further improved by pressing between very elastic cylinders causing more microcrepping. The paper may be coated with polyethylene (PE) to ensure an effective barrier against moisture, grease and bacteria. A paper sack can be made of several layers of sack paper depending on the toughness needed.
Kraft paper is produced on paper machines with moderate machine speeds. The raw material is normally softwood pulp from the kraft process.
Maintaining a high effective sulfur ratio or sulfidity is important for the highest possible strength using the kraft process.
The kraft process can use a wider range of fiber sources than most other pulping processes. All types of wood, including very resinous types like southern pine, and non-wood species like bamboo and kenaf can be used in the kraft process.
- Normal kraft paper is strong and relatively coarse. It has high tensile strength. The grammage is normally from 40–135 g/m2.
- Sack kraft paper, or just sack paper is a porous kraft paper with high elasticity and high tear resistance, designed for packaging products with high demands for strength and durability.
- Absorbent kraft paper is made with controlled absorbency, i.e., a high degree of porosity. It is made of clean low kappa hardwood kraft and has to have a good uniformity and formation.
- Spinning kraft paper is an especially strong type of kraft paper with relatively low grammage (40 g/m2). This paper requires the best possible machine direction strength and cross machine elongation. This is done by high fiber orientation on the papermachine.
- Hunting cartridge paper is a kraft paper used in shotgun shells. This paper needs a high tensile strength in the machine direction, which is the axial direction of the cartridges. In the cross direction, the cartridge is supported by the gun-pipe, but a sufficient elongation is needed. The body of the cartridge is wound of a kraft paper of 80–120 g/m2, which is further covered by an outer sheet of 60–80 g/m2 with colour and printing.
- Candy wrapping paper or twisting paper are thin 30–40 g/m2 kraft papers and is mostly flexo or offset printed. These papers requires a good strength, with highly oriented fibers. Twisting paper is mostly opaque and often supercalendered.
- Kraft paper (plastic hazard free) is used paper sacks for cement, food, chemicals, consumer goods,flour bags etc.
- Kraft paper is a cheap material for lining particle boards.
- The base paper for sandpaper is normally kraft paper.
See also 
- Derived from German Kraft, meaning "strength" in this context, due to the strength of the paper produced using this process.
- Paulapuro, Hannu (2000). "5". Paper and Board grades. Papermaking Science and Technology 18. Finland: Fapet Oy. pp. 121–122. ISBN 952-5216-18-7
- Hubbe, Martin a.; Lucian A. Lucia (2007). "The "Love-Hate" Relationship Present in Lignocellulosic Materials". BioResources 2 (4): 534–535. Retrieved 2007-09-15.[dead link][dead link]
- "The Southern Pines" (PDF). US Department of Agriculture. 1985. Retrieved 2007-09-13.
- Yam, K. L., "Encyclopedia of Packaging Technology", John Wiley & Sons, 2009, ISBN 978-0-470-08704-6
- European Kraft Paper Producers for the Flexible Packaging Industry
- European federation of multiwall paper sack manufactures
- Paper Shipping Sack Manufactureres Assn